214 Sci. Res. Essays Figure 1. Pulse velocity testing equipment (PUNDIT).use of Ultrasonic Pulse Velocity (UPV) to the non- TEST EQUIPMENTSdestructive assessment of concrete quality has been The UPV equipment (e.g. PUNDIT) includes a transducer, aextensively investigated for decades. It is more likely to receiver and an indicator for showing the time of travel from theassess the quality and characteristics of at site concrete transducer to the receiver (Figure 1) (Pundit manual 1998).and composed of measuring the transit time of an Ultrasonic pulse uses fast potential changes to create vibration thatultrasonic pulse velocity through the concrete (Solís- leads to its basic frequency. The transducer is firmly attached toCarcaño and Moreno, 2008). The velocity of the signals concrete surface to vibrate the concrete. The pulses go through thepass through in a concrete depends on the density and concrete and reach the receiver (ASTM, 2002). The pulse velocity can be determined from the followingelasticity. According to the theory of the sound equation:propagation in solids, the sound transmission velocity isdepends on the density and the elastic modulus of the V=L/T (1)concrete and it is independent of the excitation frequencythat causes the agitation. The excitation may cause where V = pulse velocity (km/s), L = path length (cm), T = transit time (µs).longitudinal (compression) waves and transverse (shear)waves in the concrete (Hobbs and Tchoketch, 2007). Based on this technique, the velocity of sound in a concrete isNumerous data and the correlation relationships between related to the concrete modulus of elasticity:the strength and pulse velocity of concrete have beenarranged. Galan (1967) reported a regression analysis topredict compressive strength of concrete based on sound (2)characteristics like UPV and estimated concrete strengthand damping constant. where, E = modulus of elasticity, ρ=density of the concrete. A particular transducer must be used in the purpose ofdetermining dynamic elastic modulus and Poisson’s ratio The transducer detects the pulses which reach first and it is usuallyof concrete and based on the wave type (longitudinal or the leading edge of the longitudinal vibration. The positions of pulse velocity measurements are categorized in, a: Opposite faces (directtransverse). There is not any standard correlation transmission), b: Adjacent faces (semi-direct transmission) or c:between concrete compressive strength and the Same face (indirect or surface transmission) which are shown inultrasonic pulse velocity and this matter was controlled by Figure 2.many aspects (Turgut, 2004). However, the value of this In this study, the direct method is used for column, semi-directmethod to estimate the quality of concrete is based on method for beam and in-direct method for slab. The latter method isthe fact that the curve slope between the two variables is suitable for quality assessment in concrete while the pulse velocity depends only on modulus of elasticity not shape of concrete.comparatively coherent. Consequently, a calibration The Schmidt Rebound Hammer (SRH), known as the Reboundcurve between compressive strength and ultrasonic pulse or Impact Hammer test is considered as a non-destructive method,velocity obtained for each concrete is needed otherwise widely used for assessing rock quality materials considering surfacenot enough dependability would be attained (Popovics rebound hardness that is related to the compressive strength. Thisand Popovics, 1997). The nature of the aggregates which test is fast, cheap and an important guide test for rock materialis one of the major aspects that is generally more description. The methodology of the SRH test is expected to ensure the trustworthy data achievement and on site or the laboratoryplentiful, rigid, and resistant part in concrete influences analysis (Amasaki, 1991). SRH includes a spring loaded piston withthis correlation and changes the elastic properties of the steel mass (Figure 3) as explained In British Code (BS1881 partconcrete (Sturrup et al., 1984). 202, 1986). The SRH as a hardness test works in a way that the
Shariati et al. 215 Figure 2. Direct (a), Semi-direct (b) Indirect (surface) transmission (c). Figure 3. Operational system of a Schmidt Rebound Hammer (SRH).rebound of an elastic material is related to its surface hardness angle of the hammer affects the result. After the impaction, theagainst the hitting material. Based on the standard, the energy rebound readings should be recorded. There is not any distinctiveattracted by the concrete is according to its strength rebound of an relationship between hardness and strength of concrete butelastic material (ACI Committee, 1988). The kinetic energy equals experimental data relationships can be obtained from a givento the energy released by the key spring of the piston in the straight concrete (Basu and Aydin, 2004). A common normalizationimpact direction which it is released onto the hammer (Basu and procedure which could be used for any type of Schmidt hammerAydin, 2004) even if this test involves impact problems and the with the same nominal design fired in any direction (Galan, 1967).related stress-wave propagation (Qasrawi, 2000). Concrete surface However, the relationship between hardness and concrete strengthshould be carefully selected and prepared to be used by polishing depends on issues affecting the concrete surface such asso that the test surface is then ground smooth. A fixed power then saturation degree, temperature, carbonation surface preparationapplies by pushing the hammer against the surface. The slope and location (Willetts, 1958; Amasaki, 1991) also the type of
216 Sci. Res. Essays Figure 4. UPV and SRH tests in site. Table 1. Concrete mix proportion. Cement Coarse aggregate Fine aggregate Water Retarder SP Ingredient (Kg/m3) (Kg/m3) (Kg/m3) (kg/m3) (ml/ m3) (ml/m3) Amount 390 1020 805 195 1150 2305aggregate, mix proportions, hammer type, and hammer inclination this research to obtain a mathematical relationship using SRH andaffect the results (Grieb, 1958). Surfaces with scaling, UPV for investigation the reinforced concrete buildings.honeycombing, high porosity, or rough texture must be avoided. Allsamples must be at the same age, moisture conditions and the TEST PROGRAMMEsame carbonation degree (Qasrawi, 2000). It is essential to take 10to 12 readings for each surface and by the existence of aggregate Main members of an existing structure including column, beam andand voids instantly under the plunger the test is sensitive (Neville slab were tested by NDT methods (Figure 4).and Brooks, 1987). Obviously by just using the SRH, the concrete surfaces reflect.Based on British Code (BS1881 part 202, 1986), the measured Material properties and test procedurenumber by rebound hammer is an indication of the first 30-mmdepth of concrete. Another research (Aydin, 2009) recommended a Concrete mix proportion (Table1) used by the constructionmethod for determining the Schmidt hammer rebound hardness. company in Malaysia respect to (M523 part 2 1993) which is theAccording to a research by Teodoru (1989), the SRH obtained Standard for specifying, production and compliance criteria for theresults are only delegate of the outer concrete layer with a ready-mixed concrete supply in Malaysia that was adopted fromthickness of 30 to 50 mm. The simplicity of obtaining the suitable British codes (BS5328, 1976).correlation data in a given instant causes the rebound hammer to The design slump would be limited from 25 to 75 mm and thebe most useful for quick surveying in large areas of similar concrete coarse aggregate used has a nominal maximum size of 19 mmtypes in the considered construction (Qasrawi, 2000). Also the while the fine aggregate has a fineness modulus of 2.70.advantages of using rebound hammer in concrete presented The relationship between compression strength of concrete(Neville, 1973) and stated that the rebound hammer test should not collected from crashing test records and estimated results frombe accepted as a replacement for compression test but another NDT’s records was established and compared. Both, the Schmidtresearcher (Bilgin et al., 2002) strongly showed the importance of Rebound Hammer (SRH) and the Ultrasonic Pulse Velocity (UPV)SRH used for mechanical excavators with gathering arms, such as tests, are only useful provided that a correlation can be developedtunnel heading machines, may extensively improve daily advance between the rebound number/ultrasonic pulse velocity readings andrates. This is a very easy test to conduct and the rebound value is a the strength of the same concrete. This study planned to adapt thegood symptom of rock characteristics and gives significant Schmidt Rebound Hammer (SRH) equipment and the Ultrasoniccorrelation with net breaking rates of rebound hammers. Pulse Velocity (UPV) tester to investigate the concrete structures in The non-destructive methods for evaluation of the actual site. A combined method for the above two tests is established incompressive strength of concrete in existing structures are based order to improve the strength estimation of concrete.on experimental relations between strength and non-destructiveparameters. Manufacturers typically give experimental relationships TEST SPECIMENSfor their own testing system of devices. Regression analysis approach is used as destructive testing in All specimens for compression test were cubes of 150 mm side
Shariati et al. 217 Figure 5. Rebound number/compressive strength calibration curve.length for concrete strength recording. The loading speed for 150 Schmidt Rebound Hammer (SRH) resultsmm side length cube was used is 13.5kN/s. The compressivestrength of hardened concrete was determined by using specimens The best fit line, which represents the relationshiptested at 1, 3, 7, and 14 days intervals. Two specimens were tested between the rebound number and the compressiveand the averaged results for each strength test at each age wereused. strength of concrete, is a straight line which has the following equation:SCHMIDT REBOUND HAMMER (SRH) TEST fc(R)=1.7206R - 26.595 (3)The rebound number was obtained by taking 36 readings forcolumn, 18 readings for beam and 24 readings for slab. Readings where, R is the rebound number.were done in a horizontal position for beam/column and verticalposition for slab as described in British codes (BS1881 part 202 The number of used data in the correlation is n = 18. The1986). The mean rebound number and mean strength obtained R2 value is found to be 93.6%, which indicates afrom compression strength test of specimens provided the data toconstruct a correlation curve. significant correlation. The 95% prediction interval is quite narrow (f c ±4.42 MPa) where most of the data values are within this interval (Figure 5). The standard error areULTRASONIC PULSE VELOCITY (UPV) TEST found to be S.E. = 2.1024.Each concrete member for UPV test was tested as described inBritish codes (EN 12504-4, 2004). The pulse velocities aremeasured in direct and semi direct method between opposite faces Ultrasonic Pulse Velocity (UPV) resultsfor column, adjacent faces for beam and indirect method for slab.The UPV readings, there are 36 readings for beam, 12 readings forcolumn and 20 readings for slab. For this test also, the mean The best-fit curve that represents the relationship has thestrength obtained from UPV and mean strength obtained from each following equation:member provided the data to achieve a correlation curve. fc(V)=15.533V - 34.358 (4)ANALYSIS AND RESULTS where, V is the ultrasonic pulse velocity.Calibration curves for each test method are drawn using The number of data used in the correlation n = 18. Theregression analysis. The correlation relation between R2 value is found to be 91.9%, which indicates apredicted and compression strength of concrete are significant correlation. The 95% prediction interval is quiterepresented by plotting the averages of rebound wider than the previous one (f c ±11.39 MPa) where thenumber/ultrasonic pulse velocity against the compressive most data values are within this interval. (Figure 6) andstrength of each member. the standard error are found to be S.E. = 3.3746.
218 Sci. Res. Essays Figure 6. Ultrasonic Pulse Velocity (UPV)/compressive strength calibration curve.Combined analysis author’s calibration curve is higher than the other ones, achieved by other researchers (Figures 7 and 8) andDependability of results was enhanced while the SRH calibration curve is almost close to thecombination of two NDT methods was used together. To manufacturer’s calibration curve but for UPV calibrationanalyze the combined method, a multiple regression was curve is the furthest one from the manufacturer’sused to predict the concrete compressive strength. calibration curve. The effect of different features such asConsequently, the results showed a significant correlation the proportions of aggregate, water/cement ratio, curingbetween compression strength, UPV and rebound could be the cause of this difference and it does notnumbers together (Mahdi Shariati, University Putra mean less confident of this method.Malaysia, M.S thesis 2008). The compressive strengthcan be predicted from the combined ultrasonic pulsevelocity and rebound number using equation 5 with R2 = CONCLUSION0.95 where the n=18 and S.E. =1.8491 and the 95%prediction interval is quite narrow (f c ±3.7 MPa): The rebound number method appears to be more 2 competent in forecasting the compression strength offc(V)=-173.04+4.07V +57.96V+1.31R (5) concrete compare than the ultrasonic pulse velocitywhere, V is the ultrasonic pulse velocity and R is the method. However, the development of calibration curvesrebound number. to conform both the Schmidt Rebound Hammer (SRH) and the UPV testing techniques for usual concrete mixes showed that the use of these two methods individually isDISCUSSION not appropriate to predict an accurate estimation for concrete strength. The use of the Schmidt ReboundObviously, the Schmidt Hammer Rebound (SRH) with Hammer (SRH) test for strength estimation of in situbest fit line has a better correlation than UPV. The concrete alone is not recommended unless using anregression model achieved from combination of two NDT available specific calibration chart.methods are more precise and closer to the experimental The use of combined methods produces moreresults to those results that were achieved from individual trustworthy results that are closer to the true values whenmethods. compared to the use of the above methods individually. An acceptable level of precision was additionallyCOMPARISON WITH OTHER PUBLISHED WORKS appreciated for concrete strength estimation. Therefore, for engineering investigation, the resulting regressionThe compressive strength of concrete predicted by the model for strength evaluation could be used securely for
Shariati et al. 219 Research by author Dreux (1985) Rebound number Figure 7. Comparison of Schmidt Rebound Hammer (SRH) test with others. Research by authorFigure 8. Comparison of Ultrasonic Pulse Velocity (UPV) test with others.
220 Sci. Res. Essaysconcrete strength estimation. Hobbs BM, Tchoketch K (2007). Non-destructive testing techniques for the forensic engineering investigation of reinforced concrete buildings. Forensic Sci. Int., 167(2-3): 167-172. Leshchinsky A (1991). Non-destructive methods Instead of specimensACKNOWLEDGMENT and cores, quality control of concrete structures, pp. 377–386. Malaysian Standards M (1993). 523 Part 2 Specification for concrete,The author highly appreciates assistance of Mr. Sina including ready-mixed concrete. Neville A (1973). Properties of concrete, Pitman London.Mirzapour Mounes for experimental assistance. Neville A, Brooks J (1987). Concrete technology. Mag. Concrete Research 39: 140. Popovics S, Popovics J (1997). A critique of the ultrasonic pulse velocityREFERENCES method for testing concrete. NDT and E International, 30(4): 260-260. Qasrawi H (2000). Concrete strength by combined nondestructiveACI Committee (1988). In-place methods for determination of strength methods simply and reliably predicted." Cement and Concrete Res., of concrete." ACI Mater. J., 85(5). 30(5): 739-746.Amasaki S (1991). Estimation of strength of concrete structures by the Solís-Carcaño R, Moreno E (2008). Evaluation of concrete made with rebound hammer." CAJ Proc. Cem. Conc., 45: 345-351. crushed limestone aggregate based on ultrasonic pulse velocity."ASTM "C 597 (2002). Standard test method for pulse velocity through Constr. Build. Mater., 22(6): 1225-1231. concrete. Annual Book of ASTM Standards 4. Sturrup V, Vecchio F, Caratin H (1984). Pulse velocity as a measure ofAydin A (2009). ISRM Suggested method for determination of the concrete compressive strength. Situ/Nondestructive Testing of Concrete, Schmidt hammer rebound hardness: Revised version. Int. J. Rock ACI SP-82: 201-227. Mech. Mining Sci., 46(3): 627-634. Teodoru G (1989). Use of simultaneous nondestructive tests to predictBasu A, Aydin A (2004). A method for normalization of Schmidt hammer the compressive strength of concrete. Special Publication, 112: 137- rebound values. Int. J. Rock Mech. Mining Sci., 41(7): 1211-1214. 152.Bilgin N, Dincer T, Copur H (2002). The performance prediction of Turgut P (2004). Research into the correlation between concrete impact hammers from Schmidt hammer rebound values in Istanbul strength and UPV values. NDT. net, 12: 12. metro tunnel drivages. Tunnelling Undergr. Space Technol., 17(3): Willetts C (1958). Investigation of the Schmidt Concrete Test Hammer., 237-247. Misc. Papers No.6-627, U.S. Army Engineer Waterways ExperimentBritish Standards Institution (1976). BS 5328 Methods for specifying Station, Vicksburg, Miss. concrete.British Standards Institution (1986). BS1881Part 202 Recommendations for surface hardness tests by the rebound hammer.British Standards Institution (2004). EN 12504-4 Testing concrete – determination of ultrasonic pulse velocity.Galan A (1967). Estimate of concrete strength by ultrasonic pulse velocity and damping constant, ACI.Grieb W (1958). Use of Swiss hammer for estimating compressive strength of hardened concrete. Highway and search Board Bulletin, 201(1): 9581.